Electrodeposited pt on three dimensional interconnected graphene as a free standing electrode for fuel cell application
Electrodeposited Pt on three-dimensional interconnected graphene as
a free-standing electrode for fuel cell application†
Thandavarayan Maiyalagan,‡ Xiaochen Dong,‡ Peng Chen* and Xin Wang*
Received 12th December 2011, Accepted 30th January 2012
A three-dimensional interconnected graphene monolith was used
as an electrode support for pulsed electrochemical deposition of
platinum (Pt) nanoparticles. Pt nanoparticles with well-deﬁned
morphology and small size can be obtained by controlling elec-
trodeposition potential and time. Electrochemical characterization
was carried out to examine the electrocatalytic activity of this
monolithic electrode towards methanol oxidation in acidic media.
The results show that the carbon material surface and structure
have a strong inﬂuence on the Pt particle size and morphology.
Compared with the three-dimensional scaffold of carbon ﬁbers,
the three-dimensional graphene when used as a free-standing
electrode support resulted in much improved catalytic activity for
methanol oxidation in fuel cells due to its three-dimensionally
interconnected seamless porous structure, high surface area and
Graphene, a two-dimensional (2D) nanomaterial with a single sheet
of carbon atoms packed in a hexagonal lattice, has recently attracted
attention due to its fascinating properties, such as high surface area,
extraordinary conductivity due to high charge carrier mobility and
capacity and excellent mechanical strength.1–4
These unique proper-
ties make graphene a promising material for energy conversion and
It is believed that developing macroscopic
three-dimensional (3D) architecture of graphene will further extend
its abilities towards these applications. There are many reports in the
literature on graphene powder as a catalyst support for fuel cells.10,11
The methods of preparation of the Pt nanoparticles and alloys on the
graphene support have attracted much interest in view of superior
electrocatalytic activity for fuel cell applications.12,13
to conventional fuel cell electrodes, these materials still suffer from
insufﬁcient Pt utilization due to the segregation by an insulating
PTFE binder in the real fuel cell electrode.
Recently, a novel 3D interconnected graphene network has been
which opens up a new promising way for the application
of graphene based materials. Exhibiting an open-pore honeycomb
structure, this 3D graphene has an exceptionally large void volume,
high surface area, high corrosion resistance and high electrical
conductivity. All these properties make it ideal as the electrode
support material for fuel cell applications. Firstly, high corrosion
resistance of the graphene material can signiﬁcantly reduce the
support corrosion problem, which has been identiﬁed as one of the
main reasons for the quick performance loss of fuel cells.15
high electrical conductivity is essential for efﬁcient electron conduc-
tion through the electrode. Compared to the powder form, the unique
monolithic nature can better maintain its conductivity by eliminating
junction resistance when used as an electrode. Thirdly, the high
surface area of the 3D graphene allows uniform and high loading of
catalysts (here, Pt nanoparticles). Lastly, the interconnected pores
may potentially offer low resistance to ﬂuid ﬂow and ensure efﬁcient
mass transfer during fuel cell operation.
In this work, the free-standing 3D graphene was examined for the
ﬁrst time as an electrode support for methanol oxidation and
compared with the free-standing carbon ﬁber (CF) material16
a similar three-dimensional structure. The present investigation
provides insights and demonstrates potentials of this material for
fuel cell applications. The 3D graphene electrode poses two major
challenges. The ﬁrst one relates to synthesizing and uniformly depos-
iting nano-sized Pt electro-catalyst throughout the three-dimensional
catalytic sites andthe proton exchange membrane. Toaddress the ﬁrst
issue, pulse electrodeposition is adopted which ensures that all the
deposited Pt nanoparticles (NPs) are electrically accessible. Further-
more, pulse electrodeposition exhibits several advantages over direct
current electrodeposition in the control of particle size, uniform
distribution and strong adhesion of the NPs on the substrate.17–19
second issue of protonic conductivity in the fuel cell electrode could be
addressed by employing a hydrophilic Naﬁon electrolyte.
Towards that end, deposition of Pt-NPs on the 3D monolithic
graphene architecture is designed and improved activity for methanol
oxidation is reported. The improved activity and stability of the
electrode were attributed to the unique 3D monolithic architecture
with outstanding conductivity and in the absence of junction resis-
tance, which leads to efﬁcient electron conduction and mass
School of Chemical and Biomedical Engineering, Nanyang Technological
University, 62 Nanyang Drive, 639798, Singapore. E-mail: WangXin@
ntu.edu.sg; ChenPeng@ntu.edu.sg; Fax: +(65) 6794 7553; Tel: +(65)
† Electronic supplementary information (ESI) available. See DOI:
‡ Both authors contributed equally to this work.
5286 | J. Mater. Chem., 2012, 22, 5286–5290 This journal is ª The Royal Society of Chemistry 2012
Dynamic Article LinksC<Journal of
Cite this: J. Mater. Chem., 2012, 22, 5286
View Article Online / Journal Homepage / Table of Contents for this issue
2.1 Synthesis of 3D graphene foams
The 3D graphene foams with continuous single and few-layer
graphenes were synthesized by chemical vapour deposition using
nickel foam as the template and ethanol as precursors.14,20
nickel foams (0.5 mm in thickness, 320 g mÀ2
in areal density) were
cut into 2 Â 2 cm and placed in a quartz tube furnace with temper-
ature gradually increased to 1000
C under H2 (25 sccm) and Ar
(50 sccm) environment. After annealing for 10 min to clean the nickel
surface, the ethanol vapour was introduced into the tube by H2/Ar
mixture gas at ambient pressure. 20 min later, the samples were
rapidly cooled to room temperature at a rate of $100
the growth process, the nickel substrates were etched away with HCl
(3 M) solution at 80
C to obtain free-standing 3D graphene foams.
2.2 Electrochemical deposition
A pulse potential proﬁle of 0 mV (500 ms)À1000 mV (200 ms)–0 mV
(500 ms) (vs. Ag/AgCl/3 M KCl) with different numbers of pulses was
applied for the Pt deposition. After electrodeposition of Pt particles
from the H2PtCl6 solution, the catalyst modiﬁed three-dimensional
graphene support (Pt/3D-graphene) was washed with de-ionized
water and then dried.
The thickness and microstructure of the 3D graphene foams were
examined by a WITec CRM200 Confocal Raman spectrophotom-
eter (laser wavelength 488 nm). The morphology of the samples
was observed by a ﬁeld-emission scanning electron microscope
(JEOL-JSM6700-FESEM). X-Ray diffraction (XRD) patterns were
collected with a Bruker D8 Advanced Diffractometer using Cu Ka
2.4 Electrochemical measurements
The electrochemical properties of the free-standing 3D graphene
electrodes were examined using an Autolab Electrochemical Working
Station in a three-electrode system in 0.5 M H2SO4 electrolyte
at room temperature. Pt gauze was used as the counter electrode,
Ag/AgCl as the reference electrode and 3D graphene as the work
electrode directly. Stable data were recorded after 20 cycles.
The potential range for cyclic voltammetry (CV) measurements was
À0.2 to +1.0 V at a scan rate of 50 mV sÀ1
3. Results and discussion
3.1. Substrate characterization
Fig. 1a provides a photograph of the obtained free standing graphene
foam which is ﬂexible and black. The monolithic and porous 3D
graphene architecture can be clearly observed in Fig. 1a and 2a. The
3D graphene was characterized by Raman spectroscopy, where
two characteristic peaks at $1560 cmÀ1
(G-band) and $2700 cmÀ1
As revealed by the integrated intensity ratio of G and 2D bands
(IG/I2D) in the Raman spectrum, the 3D graphene exhibits single-
layer and few-layer domains (Fig. 1b).22
Because IG increases
monotonically with the increasing graphene thickness whereas I2D is
relatively stable, IG/I2D scales linearly with the number of graphene
layers (up to 4 layers).23
The Raman D-band (at $1350 cmÀ1
) is originated from the
disordered carbon in graphene, and its intensity indicates the density
of defects in the as-grown graphene ﬁlm.24
The extremely weak
D-band in the Raman spectra of the free-standing 3D graphene
(Fig. 1b) demonstrates the high quality of the obtained graphene.
Fig. 2a and b show the morphology of 3D graphene and carbon
ﬁber support (carbon paper). The inset in Fig. 2a shows the surface
morphology of 3D graphene at a higher magniﬁcation. SEM analyses
reveal that the carbon paper consists of overlapped crossed ﬁbers
(Fig. 2b) and the diameter of the ﬁbers is about 5 mm. Controlling the
size and dispersion of Pt NPs on 3D graphene is critical for their
application in fuel cells. In our study, the Pt NPs with controllable size
and dispersion are achieved by controlling the pulse deposition in
aqueous solution. SEM analyses revealed that pulse deposition
(200 pulses) led to well deﬁned spherical-type Pt particles uniformly
(Fig. 2c). Control experiments by the conventional electrodeposition
technique in 1 mM H2PtCl6 + 1 M K2SO4 at À200 mV vs. SCE for
Fig. 1 (a) Photograph of 3D graphene foam and (b) typical Raman
spectra measured at different spots of 3D graphene foam reveal the
existence of single layer (1L) and few-layer (ML) domains.
Fig. 2 SEM images of the (a) 3D graphene support (b) carbon ﬁber
support (c) Pt/3 D-GN catalyst and (d) Pt/CF catalyst. Insets in (a) and
(d) are the enlarged pictures.
This journal is ª The Royal Society of Chemistry 2012 J. Mater. Chem., 2012, 22, 5286–5290 | 5287
View Article Online
leads to higher particle sizes of about 100–200 nm (ESI, Fig. S1†).
TEM images (ESI†, Fig. S2b) also conﬁrm the Pt particles on 3D
graphene. The uniform and dense distribution of smaller platinum
particles on the 3D graphene electrode substrate desirably provides
abundant catalytic sites. As a result, high electro-catalytic activity was
Fig. 2d shows a low-magniﬁcation SEM image of porous carbon
paper decorated with Pt NPs. A higher magniﬁcation SEM image
(Fig. 2d, inset) indicates that a large number of NPs, with particle sizes
observed that the dispersion of Pt NPs is more uniform and denser in
Pt/3D-graphene than in Pt/CF presumably due to the surface ﬂatness
of 3D-graphene compared to a highly curved surface of carbon ﬁber.
Therefore, 3D-graphene is proved to be a better catalyst support than
XRD analysis shown in Fig. 3 reveals that the prepared catalysts
exhibit a typical face-centered cubic (fcc) Pt lattice structure. The Pt/
3D-graphene catalyst shows a diffraction peak at $26
that the graphitic nature of 3D-graphene is still maintained after the
catalyst preparation. In contrast, the XRD pattern of the Pt/CF
paper exhibits one broad peak centered at $25.6
, indicating the
amorphous nature. The average particle sizes of Pt/3D-graphene and
Pt/CF, calculated from the (1 1 1) peak using the Debye–Scherrer
equation, are 7.89 and 13.6 nm, respectively. The particle sizes
observed by SEM are larger than those estimated from XRD,
implying that the agglomerates comprise much smaller particles,
particularly in the case of carbon ﬁber.
3.2. Intrinsic activity of Pt NPs for methanol electro-oxidation
Fig. 4a shows the cyclic voltammogram of both catalytic substrates in
nitrogen purged 0.5 M H2SO4. Pt/3D-graphene exhibits larger
double-layer capacitance than Pt/CF, reﬂecting that the electro-
chemically active surface area of 3D-graphene is signiﬁcantly larger
than that of carbon ﬁber (Fig. 4a). In addition, the electrochemically
active Pt area, determined by integrating the hydrogen adsorption
area, is found to be 58% higher for Pt/3D-graphene than for Pt/CF.
The larger Pt area in Pt/3D-graphene is ascribed to better dispersion
of Pt on 3D-graphene, which is conﬁrmed by the SEM analysis.
To evaluate the electro-catalytic activity of Pt/3D-graphene
towards methanol electro-oxidation, cyclic voltammograms were
recorded in a nitrogen purged solution of 0.5 M H2SO4 containing
1 M CH3OH at a scan rate of 50 mV sÀ1
and the current reported
was normalized by the Pt active surface area. On the forward
potential sweep (Fig. 4b), the current increased slowly at lower
potentials, and then quickly increased at potentials higher than 0.5
V. These features of the voltammogram, which are similar to those
of the Pt metal, suggest that the well dispersed Pt NPs on the 3D
graphene are electrochemically active.25
The magnitude of the peak
current density is directly proportional to the amount of methanol
oxidized at the electrode. The peak current density of the forward
anodic peaks (If) observed with 3D-graphene is approximately
1.6 mA cmÀ2
, nearly two times the peak current density of the
carbon ﬁber (0.8 mA cmÀ2
); this result suggests that 3D-graphene
plays a critical role in promoting methanol oxidation of Pt NPs. The
current density of commercial Pt/C26
catalysts is 1.39 mA cmÀ2
which is lower than the 3D graphene catalysts. The ratio of the
forward anodic peak current density (If) to the reverse anodic peak
current density (Ib) can be used to describe the tolerance of Pt
catalysts to CO and other carbonaceous species. The If/Ib ratio for
commercial Pt/C is about 0.80. The reported value of the If/Ib ratio
of commercial E-TEK catalyst is $1 (ref. 27–30) and three-dimen-
sional Pt-on-Pd bimetallic nanodendrites supported on graphene
nanosheets is 1.25 (ref. 31). In the present study, the carbon ﬁber-
supported Pt NPs have a similar If/Ib ratio as the E-TEK catalyst.
The 3D graphene-supported Pt NPs have a ratio of 2.25, suggesting
that graphene-supported Pt NPs generate a more complete oxida-
tion of methanol to carbon dioxide. Taken together, the highly
conductive Pt/3D-graphene electrode with smaller Pt NPs sizes and
better dispersion of NPs exhibits superior intrinsic activity for
Chronoamperometric measurements of Pt/3D-graphene and
Pt/CF are shown in Fig. 5, which reﬂect the activity and stability
of the catalyst to catalyse methanol. Under a given potential of 0.6 V,
Pt/3D-graphene shows a higher initial current and a slower decay of
the peak current with time, suggesting a better catalytic activity and
stability than Pt/CF.
High catalytic efﬁciency for 3D graphene-supported Pt was
achieved due to the maximization of the three-phase boundary (TPB)
in the electrode by depositing Pt NPs on the outermost surface area of
an established porous network. In our method, a free-standing 3D
graphene was constructed; Pt NPs were then electro-deposited on the
3D graphene in a liquid solution. Only those sites that are electrolyte
accessible and electron accessible can have the deposition of Pt NPs.
The advantages of a catalytic electrode made with this 3D graphene
include: (1) its unique monolithic network structure offers continuous
and multiplexing pathways for electron conduction; (2) Pt NPs are
electrodeposited on the most efﬁcient contact zones with guaranteed
electronic and electrolytic pathways in the 3D graphene; (3) the open
vacancies (pores) mostly in the meso- to macro-size range can be
effectively covered by Naﬁon electrolytes, which facilitates the
maximization of the three-phase boundary where the electrochemical
reaction takes place; (4) the high porosity of 3D graphene also
beneﬁts the mass transfer process within the catalyst layer resulting in
further improvement for Pt utilization; and (5) the Pt/3D-graphene
electrode also showed higher stability and higher conductivity.
Combining these advantages, a much improved performance for
methanol oxidation is achieved.Fig. 3 XRD patterns of Pt/3 D-GN and Pt/CF catalysts.
5288 | J. Mater. Chem., 2012, 22, 5286–5290 This journal is ª The Royal Society of Chemistry 2012
View Article Online
One additional beneﬁt of this 3D graphene is its much lighter
weight compared to the similar sized carbon ﬁber. This could be
advantageous for applications where the system weight is a critical
Platinum nanoparticles deposited on 3D graphene and carbon ﬁber
scaffold by the pulse electrodeposition method exhibit different
catalytic activity towards methanol oxidation. This difference in
catalytic activity can be attributed to the geometry difference of these
carbonaceous supports. The enhancement in the Pt/3D-graphene
catalyst is attributed to the superior electrical conductivity, large
surface area and efﬁcient mass transport, and dense coating of small
platinum nanoparticles. Detailed electrochemical characterization
shows the 3D graphene structure as a new kind of supporting
material with higher catalytic activity and stability for methanol
oxidation. The present approach can be readily extended by deco-
rating free-standing 3D graphene with nanoparticles of other noble
metals and their alloys for various electro-catalysis applications or
The authors are deeply grateful to the National Research Foundation
(Singapore) for the Competitive Research Program (2009 NRF-
CRP001-032) and the Ministry of Education (Singapore) for the
academic research fund ARC 2/10 (MOE2009-T2-2-024).
Notes and references
1 M. D. Stoller, S. Park, Y. Zhu, J. An and R. S. Ruoff, Nano Lett.,
2008, 8(10), 3498–3502.
2 Y. X. Xu and G. Q. Shi, J. Mater. Chem., 2011, 21, 3311–3323.
3 C. Mattevi, H. Kim and M. Chhowalla, J. Mater. Chem., 2011, 21,
4 C. Lee, X. Wei, J. W. Kysar and J. Hone, Science, 2008, 321(5887),
5 Y. Shao, S. Zhang, M. H. Engelhard, G. Li, G. Shao, Y. Wang, J. Liu,
I. A. Aksay and Y. Lin, J. Mater. Chem., 2010, 20, 7491–7496.
6 Y. Zhang, T. Mori, L. Niu and J. Ye, Energy Environ. Sci., 2011, 4,
7 S. Y. Wang, S. P. Jiang and X. Wang, Phys. Chem. Chem. Phys., 2011,
8 J.-J. Shi, G.-H. Yang and J.-J. Zhu, J. Mater. Chem., 2011, 21, 7343–
9 Y. Sun, Q. Wu and G. Shi, Energy Environ. Sci., 2011, 4, 1113–1132.
10 J. Hou, Y. Shao, M. W. Ellis, R. B. Moore and B. Yi, Phys. Chem.
Chem. Phys., 2011, 13, 4083–4094.
11 Y. Hu, H. Zhang, P. Wu, H. Zhang, B. Zhou and C. Cai, Phys. Chem.
Chem. Phys., 2011, 13, 15384–15402.
12 Y. G. Zhou, J. J. Chen, F. B. Wang, Z. H. Sheng and X. H. Xia,
Chem. Commun., 2010, 46, 5951–5953.
13 J.-D. Qiu, G.-C. Wang, R.-P. Liang, X.-H. Xia and H.-W. Yu, J.
Phys. Chem. C, 2011, 115, 15639–15645.
14 Z. Chen, W. Ren, L. Gao, B. Liu, S. Pei and H.-M. Cheng, Nat.
Mater., 2011, 10, 424–428.
15 X. Wang, W. Z. Li and Y. S. Yan, J. Power Sources, 2006, 158, 154–
16 S. Uhm, H. L. Lee, Y. Kwon and J. Lee, Angew. Chem., Int. Ed., 2008,
17 H. Kim and B. N. Popov, Electrochem. Solid-State Lett., 2004, 7,
18 H. Kim, N. P. Subramanian and B. N. Popov, J. Power Sources, 2004,
19 C. Coutanceau, A. F. Rakotondrainibe, A. Lima, E. Garnier,
S. Pronier, J.-M. Leger and C. Lamy, J. Appl. Electrochem., 2004,
Fig. 4 (a) Cyclic voltammograms of Pt/3D-graphene and Pt/CF catalysts in H2SO4 (scan rate: 50 mV sÀ1
) and (b) in a mixture solution of 0.5 M H2SO4
and 1 M CH3OH (scan rate: 50 mV sÀ1
Fig. 5 Chronoamperometric curves at 0.6 V for 3600 s of (a) Pt/3D-
graphene and (b) Pt/CF electro-catalysts in 0.5 M H2SO4/1 M CH3OH
solutions at 25
This journal is ª The Royal Society of Chemistry 2012 J. Mater. Chem., 2012, 22, 5286–5290 | 5289
View Article Online
20 X. Dong, W. Fang, C. Y. Su, Y. H. Chen, L. J. Li, W. Huang and
P. Chen, Carbon, 2011, 49, 3672–3678.
21 A. C. Ferrari, J. C. Meyer, V. Scardaci, C. Casiraghi, M. Lazzeri,
F. Mauri, S. Piscanec, D. Jiang, K. S. Novoselov, S. Roth and
A. K. Geim, Phys. Rev. Lett., 2006, 97, 187401–187404.
22 Y. Huang, X. Dong, Y. Shi, C. M. Li, L. J. Li and P. Chen, Nanoscale,
2010, 2, 1485–1488.
23 D. Graf, F. Molitor, K. Ensslin, C. Stampfer, A. Jungen, C. Hierold
and L. Wirtz, Nano Lett., 2006, 7, 238–242.
24 M. S. Dresselhaus, A. Jorio, M. Hofmann, G. Dresselhaus and
R. Saito, Nano Lett., 2010, 10, 751–758.
25 D. Pletcher and S. Sotiropoulos, J. Chem. Soc., Faraday Trans., 1994,
26 F. Su, J. Zeng, X. Bao, Y. Yu, J. Y. Lee and X. S. Zhao, Chem.
Mater., 2005, 17, 3960–3967.
27 V. Raghuveer and A. Manthiram, J. Electrochem. Soc., 2005, 152,
28 T. C. Deivaraj and J. Y. Lee, J. Power Sources, 2005, 142, 43–49.
29 Z. C. Wang, D. D. Zhao, G.-Y. Zhao and H. L. Li, J. Solid State
Electrochem., 2009, 13, 371–376.
30 S. Guo, S. Dong and E. Wang, Small, 2009, 5, 1869–1876.
31 S. Guo, S. Dong and E. Wang, ACS Nano, 2010, 4, 547–555.
5290 | J. Mater. Chem., 2012, 22, 5286–5290 This journal is ª The Royal Society of Chemistry 2012
View Article Online